The Effect of Four Surface Treatment Methods on the Shear Bond Strength of
Metallic Brackets to the Fluorosed Enamel
Hooman Zarif Najafi a, Vahid Moshkelgosha a, Atefeh Khanchemehr b, Akram Alizade b, Ali Mokhtar c
Orthodontic Research Center, Dept. of Orthodontics, School of Dentistry, Shiraz University of Medical Sciences, Shiraz, Iran.
b Student Research Committee, School of Dentistry, Shiraz University of Medical Sciences, Shiraz, Iran. c
School of Dentistry, Tehran Islamic Azad University of Medical Sciences, Tehran, Iran.
Received July 2014;
Received in revised form October 2014; Accepted December 2014;
Statement of the Problem: Some studies have reported the bond strength to be sig-nificantly lower in fluorotic enamels than the non-fluorosed.
Purpose: The purpose of this study was to evaluate the shear bond strength of metal-lic brackets to non-fluorosed and fluorosed teeth after different enamel conditioning.
Materials and Method: A total of 176 freshly extracted human premolars (88 non-fluorosed and 88 non-fluorosed teeth) were used in this study for bonding the metallic
brackets. Teeth with moderate fluorosis were used according to Thylstrup and
Fejereskov index (TFI). Eighty non-fluorosed and 80 fluorosed teeth (TFI=4-6) were
randomly divided into 8 equal groups of 20 teeth each. The remaining 16 teeth were
used for scanning electron microscopy observation. The enamel surface was
condi-tioned by 4 methods: acid etching for 30 sec, acid etching for 120 sec, air abrasion
followed by acid etching, and Er: YAG laser etching followed by acid etching. The
morphology of etching patterns in different groups was studied under scanning
Results: The shear bond strength of fluorosed teeth to the brackets was significantly lower than non-fluorosed ones (p= 0.003). The shear bond strength of laser-acid
groups in both non-fluorosed and fluorosed teeth was significantly lower than other
groups (p< 0.001). Weibull analysis indicated that the chance of failure under the
applied force was different between fluorosed and non-fluorosed group. The scanning
electron microscope observations revealed that the fluorosed teeth treated with
phos-phoric acid had fewer irregularities compared to non-fluorosed teeth. The most
irregu-larities were detected in the teeth conditioned with phosphoric acid for 120 seconds.
Conclusion: Fluorotic enamel adversely affects the bond strength of orthodontic brackets. None of the conditioning methods tested in this study could significantly
improve shear bond strength of metallic brackets. Er: YAG laser conditioning
fol-lowed by acid further reduced the bond strength in non-fluorosed and fluorosed teeth.
Corresponding Author: Moshkelgosha V., Orthodontic Research Center, Department of Orthodontics, School of Dentistry, Shiraz University of Medical Sciences, Shiraz, Iran. Tel: +98-71-3626193-4 Email: email@example.com
Cite this article as: Zarif Najafi H., Moshkelgosha V., Khanchemehr A., Alizade A., Mokhtar A. The Effect of Four Surface Treatment Methods on the Shear Bond Strength of Metallic
Brackets to the Fluorosed Enamel. J Dent Shiraz Univ Med Sci., 2015 September; 16(3 Suppl): 251-259.
Fluoridation is considered among the most effective
tools in prevention of dental caries.  However,
exces-sive levels of fluoride in water supplies of different
geo-graphic areas have been responsible for clinically
unde-sirable fluorosis.  Fluorosed enamel consists of an
outer hypermineralized layer which is acid-resistant and
an underlying hypomineralized porous layer. [3-4]
Cur-rently, direct bonding of brackets and attachments is one
ortho-dontic treatment.  Meanwhile, obtaining a strong and
reliable adhesive bond between the tooth enamel and
orthodontic brackets is of great importance in
orthodon-tic pracorthodon-tice. 
While the routine method for conditioning the
enamel surface is using phosphoric acid,  the
hy-permineralized enamel surface has been proved difficult
to etch.  Some studies has found the bond strength to
be significantly lower in fluorotic than the
non-fluorosed enamels, [1,9-10] while other studies declared
no difference between the two. [5-6]
Several methods of enamel surface treatment have
been recommended by different studies for
reinforce-ment of the bond strength to the fluorosed enamel.[8,
11-12] One of these methods is grinding the enamel
which results in enhanced surface roughness of the
fluorosed tooth  and might reinforce the bond
strength to enamel.  Similarly, extended enamel
conditioning with phosphoric acid can remove the acid
resistant hypermineralized surface layer. [15-16]
Air abrasion isanother method that has been
ap-plied in order to strengthen the bond strength to
fluorosed teeth.  This method, in which the enamel
surface is roughened, can be used during orthodontic
treatments. [18-19] Some investigations [20-21] also
showed that the lasers can be effective in enamel
condi-tioning. Different types of laser such as Er:YAG
(erbi-um-doped yttrium aluminum garnet), Nd:YAG
(neo-dymium-doped yttrium aluminum garnet) and ErCr:
YSGG have been used for enamel conditioning in
or-thodontics.  Er:YAG laser has been approved as an
effective tool for hard tissue ablation.  Attrill et al.
 supported the use of Er:YAG laser as an alternative
to conventional acid etching. Although, Lee et al. 
and Ferreira et al. reported that the mean bond
strength have not increased after laser etching followed
by acid etching.
To the best of our knowledge, no studies have
evaluated the effect of laser etching on the bond strength
of fluorosed teeth. Concerning the previous
controver-sial results regarding other enamel conditioning
meth-ods and high prevalence of dental fluorosis in some
regions,  it seems necessary to scrutinize the best
method of enamel surface treatment for bracket bonding
in fluorosed teeth.
The aim of this study is to compare the shear bond
strength (SBS) of metallic brackets to the fluorosed and
non-fluorosed teeth after enamel preparation by use of
four different surface conditioning methods: acid
etch-ing, prolonged etchetch-ing, air abrasion combined with acid
etching, and Er:YAG laser combined with acid etching.
Materials and Method
Choosing and grouping the experimental teeth
This in vitro study recruited 176 human premolars
ex-tracted for orthodontic reasons from the patients aged
20-40. These intact teeth had no caries, restoration, or
chipping. Half of the samples (n=88) were
non-fluorosed [Thylstrup and Fejereskov index (TFI) =0]
and the other half were moderately fluorosed (TFI=4-6).
 The fluorosed teeth were collected from endemic
areas of fluorosis in southern parts of Iran.
All samples were cleaned by ultrasonic scaler
(Dentsply International Inc.; York, USA) and were then
polished for 20 seconds with non-fluoridated pumice
and rubber cap. Finally, they were disinfected for about
24 hours through being plunged in distilled water
com-prising 0.1% thymol solution. After that, they were
ran-domly divided into 8 equal groups of 20 teeth each.
Groups 1 to 4 were non-fluorosed and groups 5 to 8
were fluorosed. The remaining 16 teeth were used for
scanning electron microscopy (SEM) observation.
Mounting and preparation of samples
By using a mounting jig, the teeth were first embedded
in a 2.6×2cm acrylic mold (Orthocryl; Dentaurum,
Ispringen, Germany). The mounting jig was used to
align the direction of debonding force parallel to the
buccal surface of the teeth during the measurement of
SBS. The buccal surfaces of the samples in groups 1
and 5 (acid-etch groups) were etched for 30 seconds
with 37% phosphoric acid (Gel etch®; 3M Unitek,
Monrovia, California, USA). After that, they were
rinsed for 20 seconds with deionized water and were
dried with oil-free air to leave a chalky white
appear-ance. In groups 2 and 6 (prolonged-etch groups), the
procedures were performed the same as what was done
in groups 1 and 5, except that the teeth were etched for
120 seconds. The buccal surfaces of the teeth in groups
3 and 7 (air-abrasion and acid-etch groups) were
sand-blasted by use of 50-µm aluminum oxide particles for 5
seconds at 40-Ib pressure with micro-etcher (Micro–
Cali-fornia, USA) held at 10-mm distance. It was followed
by acid-etching with 37% phosphoric acid for 30
se-conds before rinsing and drying the teeth. In order to
determine the etching region in groups 4 and 8
(laser-acid etch groups), the buccal surfaces of the teeth were
coated with nail varnish leaving a 4×4 mm window on
the center of the crown as the laser irradiation area.
Then the samples were irradiated with Er:YAG laser
(DELight laser system; Continuum, Santa Clara, CA,
USA) with a wavelength of 2.94 µm at 300 mj/pulse,
10pps, for 10 seconds. The laser beam application was
directed manually from 1mm distance by using a
600µm optic fiber with water spray. After laser ablation,
the teeth were etched with phosphoric acid for 30
se-conds, then rinsed with deionized water for 20 sese-conds,
and dried with oil-free air.
After preparation, an adhesive primer (Transbond XT;
3m Unitek, Monrovia, Calif, USA) was applied to the
etched surfaces of the samples in all groups. The
adhe-sive paste was applied to the Ormco Mini 2000
(Ormco crop; Glendora, California, USA) premolar
metal brackets (with mean surface area of 9.63mm2).
The brackets were positioned on the teeth and seated
with firm pressure to minimize the thickness of resin
film. A probe was used to remove excess resin and
then the teeth were light cured for 20 seconds by
Ortholux LED (3M Unitek; Monrovia, California,
Measurement of the shear bond strength
Before shear testing, all samples were kept in distilled
water for 48 hours at room temperature. In order to
de-termine the SBS, a mechanical testing machine (Instron
Corp; Canton, Massachusetts, USA) applied an
occluso-cervical force to the upper surface of the bracket
be-tween the bracket base and the upper wing. SBS was
measured at a crosshead speed of 0.5 mm/ minute. The
maximum force needed for bracket debonding was rec-
orded in Newton (N) and the SBS was calculated
through dividing the force value by the bracket base
area (1 MPa = 1 N/mm2).
Adhesive remnant index (ARI)
After the experiment, an operator analyzed the brackets
and teeth under a light stereomicroscope (Olympus SZ
6045 TR Zoomstere; Olympus Optical Co., Osaka,
Ja-pan) at 10X to determine the adhesive remnant index
(ARI) according to Artun and Bergland.  The
scor-ing criteria of the index were as (0) when no adhesive
was remaining on the tooth surface, (1) when less than
half the adhesive was remaining, (2) when more than
half the adhesive was remaining, and (3) when the entire
adhesive was remaining.
Scanning electron microscopy (SEM) observation
The roots were cut and then facial surfaces were treated
similar to the enamel preparation that was performed for
each of the 8 groups; 2 teeth for each enamel
condition-ing method. The prepared samples were washed with
acetone solution for 10 minutes. Then, the enamel
sur-faces were sputter-coated with gold (SC-701AT; quick
Auto coater, Sanyu Electron Inc, Tokyo, Japan) and
observed under a SEM (JSM 5600 LV; JEOL, Tokyo,
Japan) at 20KW and 1500X magnification.
The mean, standard deviation, minimum and maximum
values were measured for all test groups. Two-way
ANOVA was used to compare SBS among the groups.
Weibull analysis was done to calculate the Weibull
modulus, characteristic strength, and the required stress
for 5% and 10% probabilities of bond failure. The
Chi-square test was used to determine significant differences
in the ARI scores among the groups. The statistical tests
were performed with SPSS software, version 17.0
(SPSS Inc; Chicago, Illinois, USA), with the
signifi-cance level set at 0.05.
Table 1: Two-way ANOVA on the force (MPa) required for debonding the metal brackets from the enamel surface
Source of variation Sum of Squares df* Mean Square F ratio P
Fluorosis (or type of enamel) 117.056 1 117.056 9.371 .003
Methods 1579.698 3 526.566 42.155 .000
Fluorosis× Methods 17.248 3 5.749 .460 .710
Error 1898.670 152 12.491
Corrected Total 3612.672 159
* df: degree of freedom
Table 2: The mean shear bond strength, standard deviation (SD), minimum and maximum values, and Weibull parameters for each group (n=20)
Study groups Mean
(MPa) SD Minimum Maximum
Shear stress at 5%
probabil-ity of failure (MPa)
Shear stress at 10%
probabil-ity of failure (MPa) Non-Fluorosed teeth
Acid etch 15.30 4.72 8.55 23.68 3.38 0.98 17.04 7.02 8.76 prolonged etch 17.85 3.40 11.47 22.12 5.28 0.99 19.61 11.18 12.81 Airabrasion+acid 16.87 3.10 11.73 21.18 5.53 0.98 17.60 10.29 11.72 Laser+acid 9.06٭ 1.83 6.70 12.25 5.18 0.95 9.88 5.57 6.35 fluorosed teeth
Acid etch 13.19 3.04 8.65 18.28 4.48 0.98 14.53 7.49 8.79 prolonged etch 16.12 4.66 9.19 24.40 3.57 0.98 18.04 7.84 9.60 Airabrasion+acid 14.51 4.11 7.86 21.18 3.59 0.99 12.46 5.45 6.66 Laser+acid 8.42٭ 2.30 5.77 13.08 3.91 0.94 9.04 4.23 5.04 ٭ shows statistically significant difference (p< 0.05) among the groups
Shear bond strength
According to the results of two-way ANOVA test as
displayed in Table1, the SBSinthe fluorosed teeth was
significantly lower than non-fluorosed teeth (p< 0.05).
Table 2 represents the SBS measurements including the
mean, standard deviation, minimum and maximum
val-ues. The highest mean SBS was observed in prolonged
etched groups (17.85±3.40MPa and 16.12±4.66MPa for
non-fluorosed and fluorosed teeth, respectively). While,
the lowest mean SBS was observed in the laser-acid
etch groups for both non-fluorosed (9.06±1.83MPa) and
fluorosed teeth (8.42±2.30 MPa). Post-hoc Tukey test
revealed a significant difference between laser-acid etch
groups and other groups in fluorosed and non-fluorosed
teeth (p< 0.001). However, no significant difference was
found among other groups (p> 0.05). Weibull data are
also shown in Table 2. Generally, the non-fluorosed
teeth had higher values of modulus when compared
with fluorosed teeth. Characteristic bond strengths in
this study ranged from 9.04 MPa in fluorosed teeth
treated by laser followed by acid to 19.61MPa in
non-fluorosed teeth treated by acid for 120 seconds,
expect-ing that 63.21% of the brackets with this bond strength
would fail.  The high values of correlation
coeffi-cient in the non-fluorosed prolonged etched group and
fluorosed air abrasion-acid group (99%) demonstrated
that the data strictly fitted the Weibull distribution
Scanning electron microscopy (SEM) observation
SEM images of enamel surfaces treated with different
methods in both non-fluorosed and fluorosed teeth are
shown in figure 1. The fluorosed teeth, treated by
phos-phoric acid for 30 seconds showed fewer irregularities
compared with non-fluorosed teeth (Figures 1a and 1e).
Most irregularities were observed in the samples
condi-tioned with phosphoric acid for 120 seconds (Figures 1b
and 1f). Laser-acid etched teeth showed an indistinct
Table 3: Distribution of adhesive remnant index (ARI) scorings in the study groups
Study groups ARI scores
0 1 2 3 Sum
Acid etch 7(35%) 7(35%) 3(15%) 3(15%) 20(100%)
Prolonged etch 5(25%) 7(35%) 5(25%) 3(15%) 20(100%)
Airabrasion+acid 8(40%) 7(35%) 3(15%) 2(10%) 20(100%)
Laser+acid 15(75%) 3(15%) 2(10%) 0(0%) 20(100%)
Acid etch 8(40%) 7(35%) 3(15%) 2(10%) 20(100%)
Prolonged etch 5(25%) 3(15%) 3(15%) 9(45%) 20(100%)
Airabrasion+acid 3(15%) 7(35%) 3(15%) 7(35%) 20(100%)
Figure 1: Scanning electron microscope images of non-fluorosed enamel surfaces (A, B, C, D) and fluorosed enamel surfaces (E, F, G, H): A and E: acid etch for 30 seconds, B and F: acid etch for 120 seconds, C and G: air abrasion followed by acid etch, D and H: laser ablated followed by acid etch. (Magnification ×1500) (The pointers show surface cracks created by laser).
etch pattern with surface cracking (Figures 1d and 1h).
Adhesive remnant index (ARI)
Modes of failure following the SBS test are
summa-rized in Table 3. Chi-square test revealed a significant
difference among the groups in terms of bond failure
(p< 0.001). There were 90% and 100% frequency of
ARI scores 0 and 1 in laser-acid etched groups in
non-fluorosed and non-fluorosed teeth, respectively. But in
oth-er groups, the frequency of ARI scores was scattoth-ered.
In this study the teeth were categorized according to
the TFI.  This index shows relevance among the
clinical form of fluorosis and the pathologic alterations
in human teeth and is one of the best indices for
as-sessment of severity of fluorosis. The samples
were obtained from patients aged 20-40 according to
Ateyah and Akpata  who reported the bond strength
to be significantly different between the patients under
or above 40 years old.
The findings of this study demonstrated that SBS
was significantly lower in fluorosed teeth compared
with the non-fluorosed teeth (p=0.003). This may be
related to the acid resistant superficial layer of the
fluorosed teeth. In agreement with our results, some
investigations [1, 9-10] indicated that there was a
sig-nificant difference in the bond strength of fluorosed
and non-fluorosed teeth. Although, Ng’ang’a et al. 
and Isci et al.  found no differences in the bond
strength of orthodontic brackets between fluorosed and
non-fluorosed teeth etched with phosphoric acid. In
our study, moderate fluorotic teeth extracted from the
patients aged 20-40 years old were assessed; while the
age range of patients and the fluorosis severity were
different in the study conducted by Ng’ang’a et al. 
and Isci et al.  Moreover, in contrast to the present
study, Ng’ang’a et al.  used tensile force for
meas-urement of the bond strength.
In our study, the highest mean SBS on
debond-ing of both fluorosed and non-fluorosed teeth was
found in prolonged etched groups, followed by air
abrasion-acid etch groups. The laser-acid etch groups
exhibited the lowest mean SBS on debonding (Table
2). In the prolonged etched groups, the etching time
was raised up from 30 to 120 seconds to overcome the
acid resistant layer and improving bond strength in the
fluorosed teeth.  Opinya and Pameijer 
evaluat-ed the effect of prolongevaluat-ed etching of enamel on the
bond strength of fluorosed teeth. They reported that
extended enamel conditioning with phosphoric acid
(120 seconds) could improve the bond strength in
fluorosed teeth. Similarly, Ateyah and Akpata 
re-ported that increasing the etching time to 120 seconds
mild and moderate fluorosed teeth of the patients aged
less than 40 years; however, this was not the case in
the teeth of older patients. But, findings of our study
demonstrated that increasing the etching time from 30
to 120 seconds did not result in a significant increase
in the SBS of orthodontic brackets for moderate
fluorosed and non-fluorosed premolar teeth. Similar
results were obtained by Silva Benitez et al.  who
etched severely fluorosed molar teeth for 150 seconds.
The different results yielded by different studies are
probably due to the various severities of fluorosis and
different etching time used in these studies. [8, 15]
Ateyah and Akpata  used both anterior and posterior
teeth (incisor, premolar, and molar) in their study and
found that the fluoride content varied among different
types of the teeth.  In addition, they grinded to
flat-ten the hypermineralized surface layer before acid
etching. The differences between the findings of
At-eyah and Akpata  and our study may be related to
the different techniques employed as mentioned above.
The findings of the current study showed that air
abrasion followed by acid etching could increase SBS
value compared with acid etching alone for both
fluorosed and non-fluorosed teeth; although this
dif-ference was not statistically significant. Silva-Benitez
et al.  detected that the use of air abrasion
fol-lowed by acid in severe fluorosis provided adequate
SBS for fixed orthodontic appliance, but the use of this
treatment could not improve bond strength in case of
moderate fluorosis. Suma et al.  stated that
com-bining air abrasion with acid etching created greater
SBS than acid etching alone in moderate to severe
dental fluorosis regardless of the adhesion system
used. They used air abrasion at air pressure of 80 PSI,
and the teeth were etched for 60 seconds after air
abra-sion. The duration of acid etching and air pressure
employed in this study was higher than our study and
these may be the factors responsible for different result.
Findings of the current study demonstrated that
bond strengths were significantly weaker when the tooth
surfaces were prepared with the Er:YAG laser followed
by acid etch compared with other enamel surface
treat-ments; it was in line with the findings of Lee et al. 
This might be due to the reduced surface area and pore
volume in the enamel surface after laser ablation. 
The lower bond strength observed in the laser followed
by acid groups compared with acid alone in our study
might be attributed to the acid resistant layer created in
enamel surface after laser application as indicated in
some investigations. [30-31] Some studies suggested
that laser ablation could create modifications in
chemi-cal and crystalline structure. Reduction of carbonate
amends the crystalline structure and subsequently
caus-es rcaus-esistance of enamel to acid dissolution. [30-31] This
may be a factor for lower bond strength in laser-acid
etch groups compared with acid etch groups. Although,
Apel et al.  and Chimello et al.  found that
enamel demineralization was not significantly different
between Er:YAG laser and unlased teeth. Another
ex-planation was presented by Ferreira et al.  who
con-cluded that the residual thermal energy after Er:Yag
laser-irradiation could change the structure of tooth
sur-face by melting and packing the tooth components
simi-lar to that of glazing, and this change remained even
after different acid etching times.  In contrast to our
results, Dunn et al.  showed that laser followed by
acid created better etch pattern and this pattern could be
more effective for bonding. The histological
investiga-tion showed that different energies of Er:YAG laser
could affect the quality of the resultant etched surface.
Therefore, the energy employed in different studies.
[23-34] may be a causing factor for different results.
The Weibull analysis is a suitable means for
pre-dicting the likelihood of failure of bracket bonding.
 The results of Weibull analysis in our study
showed that the Weibull modulus of non-fluorosed
teeth was generally higher than that of fluorosed teeth
(Table 2). Higher Weibull modulus in the
non-fluorosed teeth demonstrated high homogeneity of
SBS values in these teeth.  Moreover, mean shear
force at 5-10% probability of bond failure can be more
clinically relevant than the mean strength values or
high values.  Acceptable bond strength at 5%
probability of failure is at least 5.4 MPa.  In the
present study, the SBS of fluorosed teeth conditioned
with laser followed by acid showed a lower shear
stress level than 5.4 MPa at the 5% chance of failure.
According to these findings it can be affirmed that
laser followed by acid etching cannot be a good choice
for enamel preparation.
Our SEM observations revealed that the
pat-tern where the prism cores were eliminated and the
adjacent zone did not conform to the prism structure
(Figure 1a).However, this etching time for fluorosed
teeth, that are more resistant to acid, created less
roughness in the enamel surface (Figure 1e). The
low-er microporosities in the fluorosed enamel leads to
weaker bond in these teeth. This claim is supported by
some previous studies [16,39] which showed that
higher concentration of fluoride in teeth resulted in
more resistance to acid etching and lower surface
ir-regularity. Both the non-fluorosed and fluorosed
enamels conditioned for 120 seconds showed very
irregular surfaces with definite prominences and dents
(Figures 1b and 1f). The non-fluorosed enamel treated
with air abrasion and subsequent acid etching showed
not only an irregular surface, but also a large number
of holes probably created by the aluminum oxide
(Fig-ure 1c). The fluorosed enamel conditioned with air
abrasion and subsequent acid etching displayed just
the air abrasion effect (holes created by aluminum
oxide) (Figure 1g). According to Olsen et al.,  this
loss of enamel by aluminum oxide was irreversible,
but with acid etching, organic component remained
intact and it allowed the tooth surface to be
remineral-ized. Laser-ablated enamels are seen in Figures 1d and
1h. These images indicate that laser cannot create
dis-tinct etch pattern in the enamel surface. Moreover, the
residual thermal energy of Er:YAG laser leads to
sur-face cracking and molten sursur-face globules of enamel.
Surface cracking created by laser can decrease the
bond strength: [34, 41] and the bond strength data
from the present study appeared to support this
ARI evaluations showed that the de-bonded
brackets in the laser-acid etch groups were separated
from the resin-enamel interface. This type of bond
failure was significantly different from the other types
of bond failure occurred in other groups (p< 0.001).
These results are similar to what was found by
Mar-tinez-Insua et al.  and Kameyama et al. regarding
the fracture pattern.  We expected that this enamel
preparation might not be able to give adequate surface
wetting. In this fracture pattern, it is easy to remove
the adhesive resin from the tooth surface; however, the
probability of bond failure increases at low levels of
In conclusion, findings of the present study showed
that enamel fluorosis significantly decreased the bond
strength of orthodontic brackets. It was also found that
none of the applied methods of prolonged etching, air
abrasion combined with acid etching, and laser
com-bined with acid etching could improve the SBS of
me-tallic brackets in these teeth. Moreover, Er:YAG laser
followed by acid etching significantly reduced the SBS
when compared with the control acid etch group.
Future clinical investigations are recommended for
enhancement of the bond strength in the moderate and
also severely fluorosed teeth. Further studies are also
required to be carried out on the use of other laser
en-ergy parameters for obtaining an acceptable prepared
surface for bonding.
The authors thank the Vice-chancellery of Shiraz
Uni-versity of Medical Science for supporting this research
(Grant No. 92-6368). This article is based on the thesis
by Dr. A. Alizadeh and Dr. A. Khanchemehr. The
au-thors also thank Dr M. Vossoughi and Dr. M. Salehi at
Dental Research Development Center, Shiraz School
of Dentistry, for their help with the statistical analysis
and Dr. Sh. Hamedani (DDS, MSc) for his editorial
assistance. The authors also would like to thank the
staff of Clinical Research Development Center of
Namazi Hospital for their kind help.
Conflict of Interest
 Shida K, Kitasako Y, Burrow MF, Tagami J. Microshe- ar bond strengths and etching efficacy of a two-step self-etching adhesive system to fluorosed and non-fluorosed enamel. Eur J Oral Sci. 2009; 117: 182-186.
 Ermiş RB, Gokay N. Effect of fluorosis on dentine shear bond strength of a self-etching bonding system. J Oral Rehabil. 2003; 30: 1090-1094.
adhesion promoters on the shear bond strengths of or-thodontic brackets to fluorosed enamel. Eur J Orthod. 2009; 31: 276-280.
 Ng'ang'a PM, Ogaard B, Cruz R, Chindia ML, Aasrum E. Tensile strength of orthodontic brackets bonded di-rectly to fluorotic and nonfluorotic teeth: an in vitro comparative study. Am J Orthod Dentofacial Orthop. 1992; 102: 244-250.
 Isci D, Sahin Saglam AM, Alkis H, Elekdag-Turk S, Turk T. Effects of fluorosis on the shear bond strength of orthodontic brackets bonded with a self-etching primer. Eur J Orthod. 2011; 33: 161-166.
 Torres-Gallegos I, A Martinez-Castañon G, Loyola-Rodriguez JP, Patiño-Marin N, Encinas A, Ruiz F, Anusavice K. Effectiveness of bonding resin-based com-posite to healthy and fluorotic enamel using total-etch and two self-etch adhesive systems. Dent Mater J. 2012; 31: 1021-1027.
 Ateyah N, Akpata E. Factors affecting shear bond strength of composite resin to fluorosed human enamel. Oper Dent. 2000; 25: 216-222.
 Adanir N, Türkkahraman H, Güngör AY. Effects of fluorosis and bleaching on shear bond strengths of or-thodontic brackets. Eur J Dent. 2007; 1: 230-235. Gungor AY, Turkkahraman H, Adanir N, Alkis H.
Ef-fects of fluorosis and self etching primers on shear bond strengths of orthodontic brackets. Eur J Dent. 2009; 3: 173-177.
Miller RA. Bonding fluorosed teeth: new materials for old problems. J Clin Orthod. 1995; 29: 424-427. Duan Y, Chen X, Wu J. Clinical comparison of bond
failures using different enamel preparations of severely fluorotic teeth. J Clin Orthod. 2006; 40: 152-154. Ratnaweera PM, Nikaido T, Weerasinghe D, Wettasin-
ghe KA, Miura H, Tagami J. Micro-shear bond strength of two all-in-one adhesive systems to unground fluorosed enamel. Dent Mater J. 2007; 26: 355-360. Ermis RB, De Munck J, Cardoso MV, Coutinho E, Van
Landuyt KL, Poitevin A, et al. Bonding to ground versus unground enamel in fluorosed teeth. Dent Mater. 2007; 23: 1250-1255.
Silva-Benítez EL, Zavala-Alonso V, Martinez-Castanon GA, Loyola-Rodriguez JP, Patiño-Marin N, Ortega-Pedrajo I, et al. Shear bond strength evaluation of bond-ed molar tubes on fluorotic molars. Angle Orthod. 2013; 83: 152-157.
Opinya GN, Pameijer CH. Tensile bond strength of fluorosed Kenyan teeth using the acid etch technique. Int Dent J. 1986; 36: 225-229.
Kwon YH, Kwon OW, Kim HI, Kim KH. Nd:YAG laser ablation of enamel for orthodontic use: tensile bond strength and surface modification. Dent Mater J. 2003; 22: 397-403.
Pakshir HR, Zarif Najafi H, Hajipour S. Effect of enamel surface treatment on the bond strength of metallic brack-ets in rebonding process. Eur J Orthod. 2012; 34: 773-777.
Suma S, Anita G, Chandra Shekar BR, Kallury A. The effect of air abrasion on the retention of metallic brackets bonded to fluorosed enamel surface. Indian J Dent Res. 2012; 23: 230-235.
DC Attrill, SR Farrar, TA King, MR Dickinson, RM Davies, AS Blinkhorn. Er: YAG (λ= 2.94 µm) laser etch-ing of dental enamel as an alternative to acid etchetch-ing. Lasers in Medical Science. 2000; 15: 154-161.
Fuhrmann R, Gutknecht N, Magunski A, Lampert F, Diedrich P. Conditioning of enamel with Nd:YAG and CO2 dental laser systems and with phosphoric acid. An in-vitro comparison of the tensile bond strength and the morphology of the enamel surface. J Orofac Orthop. 2001; 62: 375-386.
Poosti M, Jahanbin A, Mahdavi P, Mehrnoush S. Porce-lain conditioning with Nd:YAG and Er:YAG laser for bracket bonding in orthodontics. Lasers Med Sci. 2012; 27: 321-324.
Lee BS, Hsieh TT, Lee YL, Lan WH, Hsu YJ, Wen PH, et al. Bond strengths of orthodontic bracket after acid-etched, Er:YAG laser-irradiated and combined treatment on enamel surface. Angle Orthod. 2003; 73: 565-570. Ferreira LS, Apel C, Francci C, Simoes A, Eduardo CP,
Gutknecht N. Influence of etching time on bond strength in dentin irradiated with erbium lasers. Lasers Med Sci. 2010; 25: 849-854.
Thylstrup A, Fejerskov O. Clinical appearance of dental fluorosis in permanent teeth in relation to histologic changes. Community Dent Oral Epidemiol. 1978; 6: 315-328.
Artun J, Bergland S. Clinical trials with crystal growth conditioning as an alternative to acid-etch enamel pre-treatment. Am J Orthod. 1984; 85: 333-340.
eramic structures. Dent Mater. 2003; 19: 662-669. Vieira AP, Hancock R, Limeback H, Maia R, Grynpas
MD. Is fluoride concentration in dentin and enamel a good indicator of dental fluorosis? J Dent Res. 2004; 83: 76-80.
Ying D, Chuah GK, Hsu CY. Effect of Er:YAG laser and organic matrix on porosity changes in human enam-el. J Dent. 2004; 32: 41-46.
Liu JF, Liu Y, Stephen HC. Optimal Er:YAG laser energy for preventing enamel demineralization. J Dent. 2006; 34: 62-66.
Liu Y, Hsu CY. Laser-induced compositional changes on enamel: a FT-Raman study. J Dent. 2007; 35: 226-230. Apel C, Meister J, Schmitt N, Gräber HG, Gutknecht N.
Calcium solubility of dental enamel following sub-ablative Er:YAG and Er:YSGG laser irradiation in vitro. Lasers Surg Med. 2002; 30: 337-341.
Chimello DT, Serra MC, Rodrigues AL Jr, Pécora JD, Corona SA. Influence of cavity preparation with Er:YAG Laser on enamel adjacent to restorations sub-mitted to cariogenic challenge in situ: a polarized light microscopic analysis. Lasers Surg Med. 2008; 40: 634-643.
Dunn WJ, Davis JT, Bush AC. Shear bond strength and SEM evaluation of composite bonded to Er:YAG laser-prepared dentin and enamel. Dent Mater. 2005; 21: 616-624.
Nkenke E, Hirschfelder U, Martus P, Eberhard H. Eval-uation of the bond strength of different bracket-bonding
systems to bovine enamel. Eur J Orthod. 1997; 19: 259-270.
Klocke A, Kahl-Nieke B. Effect of debonding force direction on orthodontic shear bond strength. Am J Or-thod Dentofacial Orthop. 2006; 129: 261-265.
Baran GR, McCool JI, Paul D, Boberick K, Wunder S. Weibull models of fracture strengths and fatigue behav-ior of dental resins in flexure and shear. J Biomed Mater Res. 1998; 43: 226-233.
Littlewood SJ, Mitchell L, Greenwood DC. A random-ized controlled trial to investigate brackets bonded with a hydrophilic primer. J Orthod. 2001; 28: 301-305. Kochavi D, Gedalia I, Anaise J. Effect of conditioning
with fluoride and phosphoric acid on enamel surfaces as evaluated by scanning electron microscopy and fluoride incorporation. J Dent Res. 1975; 54: 304-309.
Olsen ME, Bishara SE, Damon P, Jakobsen JR. Compar-ison of shear bond strength and surface structure be-tween conventional acid etching and air-abrasion of hu-man enamel. Am J Orthod Dentofacial Orthop. 1997; 112: 502-506.
Martínez-Insua A, Da Silva Dominguez L, Rivera FG, Santana-Penín UA. Differences in bonding to acid-etched or Er:YAG-laser-treated enamel and dentin sur-faces. J Prosthet Dent. 2000; 84: 280-288.